# Modeling elastic and plastic deformations in ... grant/Papers/PhysRevE_70_ Modeling elastic

date post

25-May-2020Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of Modeling elastic and plastic deformations in ... grant/Papers/PhysRevE_70_ Modeling elastic

Modeling elastic and plastic deformations in nonequilibrium processing using phase field crystals

K. R. Elder1 and Martin Grant2 1Department of Physics, Oakland University, Rochester, Michigan 48309-4487, USA

2Physics Department, Rutherford Building, 3600 rue University, McGill University, Montréal, Québec, Canada H3A 2T8 (Received 26 June 2003; revised manuscript received 7 May 2004; published 19 November 2004)

A continuum field theory approach is presented for modeling elastic and plastic deformation, free surfaces, and multiple crystal orientations in nonequilibrium processing phenomena. Many basic properties of the model are calculated analytically, and numerical simulations are presented for a number of important applications including, epitaxial growth, material hardness, grain growth, reconstructive phase transitions, and crack propagation.

DOI: 10.1103/PhysRevE.70.051605 PACS number(s): 81.15.Aa, 05.70.Ln, 64.60.My, 64.60.Cn

I. INTRODUCTION

Material properties are often controlled by complex mi- crostructures that form during nonequilibrium processing. In general terms the dynamics that occurs during the processing is controlled by the nature and interaction of the topological defects that delineate the spatial patterns. For example, in spinodal decomposition, the topological defects are surfaces that separate regions of different concentration. The motion of these surfaces is mainly controlled by the local surface curvature and nonlocal interaction with other surfaces or boundaries through the diffusion of concentration. In con- trast, block-copolymer systems form lamellar or striped phases and the topological defects are dislocations in the striped lattice. In this instance the defects interact through long-range elastic fields.

One method for modeling the topological defects is through the use of “phase fields”[1]. These can be thought of as physically relevant fields(such as concentration, density, magnetization, etc.) or simply as auxiliary fields constructed to produce the correct topological defect motion. In con- structing phenomenological models it is often convenient to take the former point of view, since physical insight or em- pirical knowledge can be used to construct an appropriate mathematical description. In this paper the construction of a phase field model for the dynamics of crystal growth that includes elastic and plastic deformations[2] is described. The model differs from other phase field approaches to elas- ticity [3–9] in that the model is constructed to produce phase fields that are periodic. This is done by introducing a free energy that is a functional of the local-time-averaged density field, rsrW ,td. In this description the liquid state is represented by a uniformr and the crystal state is described by ar that has the same symmetry as a given crystalline lattice. This description of a crystal has been used in other contexts [10,11], but not previously for describing material processing phenomena. For simplicity this model will be referred to as the phase field crystal(PFC) model.

This approach exploits the fact that many properties of crystals are controlled by elasticity and symmetry. As will be discussed in later sections, any free energy functional that is minimized by a periodic field naturally includes the elastic energy and symmetry properties of the periodic field. Thus

any property of a crystal that is determined by symmetry (e.g., the relationship between elastic constants, number and type of dislocations, low-angle grain boundary energy, coin- cident site lattices, etc.) is also automatically incorporated in the PFC model. The model differs from standard phase field models in that the field to be considered(the time-averaged density) is only averaged in time and not in space. As will be discussed in later sections this formulation allows a descrip- tion of systems on diffusive time scales and interatomic length scales. In this sense the model bridges a molecular description(i.e., molecular dynamics) and a continuum field theory.

The purpose of this paper is to introduce and motivate this modeling technique, discuss the basic properties of the model, and present several applications to technologically important nonequilibrium phenomena. In the remainder of this section a brief introduction to phase field modeling tech- niques for uniform and periodic fields is discussed and re- lated to the study of generic liquid-crystal transitions. In the following section a simplified PFC model is presented and the basic properties of the model are calculated analytically. This includes calculation of the phase diagram, linear elastic constants, and the vacancy diffusion constant.

In Sec. III the PFC model is applied to a number of inter- esting phenomena including the determination of grain boundary energies, liquid-phase epitaxial growth, and mate- rial hardness. In each of these cases the phenomena are stud- ied in some detail and the results are compared with standard theoretical results. At the end of this section sample simula- tions of grain growth, crack propagation, and a reconstruc- tive phase transition are presented to illustrate the versatility of the PFC model. Finally a summary of the results is pre- sented in Sec. IV.

A. Uniform fields and elasticity

Many nonequilibrium phenomena that lead to dynamic spatial patterns can be described by fields that are relatively uniform in space, except near interfaces where a rapid change in the field occurs. Classic examples include order- disorder transitions(where the field is the sublattice concen- tration), spinodal decomposition(where the field is concen- tration) [12], dendritic growth[13], and eutectics[14]. To a

PHYSICAL REVIEW E 70, 051605(2004)

1539-3755/2004/70(5)/051605(18)/$22.50 ©2004 The American Physical Society70 051605-1

large extent the dynamics of these phenomena is controlled by the motion and interaction of the interfaces. A great deal of work has gone into constructing and solving models that describe both the interfaces(“sharp interface models”) and fields (“phase field models”). Phase-field models based on free-energy functionals are constructed by considering sym- metries and conservation laws and lead to a relatively small (or generic) set of sharp interface equations[15].

To make matters concrete consider the case of spinodal decomposition in AlZn. If a high-temperature homogeneous mixture of Al and Zn atoms is quenched below the critical temperature, small Al- and Zn-rich zones will form and coarsen in time. The order parameter field that describes this phase transition is the concentration field. To describe the phase transition a free energy is postulated(i.e., made up) by consideration of symmetries. For spinodal decomposition the free energy is typically written as follows:

F =E dVffsfd + Ku¹W fu2/2g, s1d where fsfd is the bulk free energy and must contain two wells, one for each phase(i.e., one for Al-rich zones and one for Zn-rich zones). The second term in Eq.(1) takes into account the fact that gradients in the concentration field are energetically unfavorable. This is the term that leads to a surface tension(or energy/length) of domain walls that sepa- rate Al and Zn-rich zones. The dynamics is postulated to be dissipative and act such that an arbitrary initial condition evolves to a lower-energy state. These general ideas lead to the well-known equation of motion

] f

] t = − Gs− ¹2da

dF df

+ hc, s2d

whereG is a phenomenological constant. The Gaussian ran- dom variablehc is chosen to recover the correct equilibrium fluctuation spectrum and has zero mean and two-point corre- lation:

khcsrW,tdhcsrW8,t8dl = GkBTs¹2dadsrW − rW8ddst − t8d. s3d

The variablea is equal to 1 iff is a conserved field, such as concentration, and is equal to 0 iff is a nonconserved field, such as sublattice concentration.

A great deal of physics is contained in Eq.(2) and many papers have been devoted to the study of this equation. While the reader is referred to[12] for details, the only sa- lient points that will be made here is that(1) the gradient term and double-well structure offsfd in Eq. (1) lead to a surface separating different phases and(2) the equation of motion of these interfaces is relatively independent of the form of fsfd. For example it is well known[12,15,16] that if f is nonconserved, the normal velocityVn of the interface is given by

Vn = k + A, s4d

wherek is the local curvature of the interface andA is di- rectly proportional to the free-energy difference between the two phases. Iff is conserved, then the motion of the inter- face is described by the following set of equations[15]:

Vn = n̂ · ¹W fms0+d − ms0−dg,

ms0d = d0k + bVn

] m/] t = D¹2m, s5d

wherem;dF /df is the chemical potential,d0 is the capil- lary length,b is the kinetic undercooling coefficient,n̂ is a unit vector perpendicular to the interface position,D is the bulk diffusion constant, and 0+ and 0− are positions just ahead and behind the interface, respectively.

It turns out that Eqs.(4) and(5) always emerge when the bulk free energy contains two wells and the local free energy increases when gradients in the order parameter field are present[15]. In this sense, Eqs.(4) and(5) can be thought of as generic or universal features of systems that contain do- main walls or surfaces. As will be discussed in the next sub- section, a different set of generic features arises when the field prefers to be periodic in space. Some generic features of periodic systems are that they naturally contain an elastic energy, are anisotropic, and have defects that are topologi- cally identical to those found in crystals. A

Recommended

*View more*